HAL Id: hal-01153244
Submitted on 19 May 2015
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Characterization of commercial supercapacitors for low
Etsuro Iwama, Pierre-Louis Taberna, Philippe Azais, Laurent Brégeon,
To cite this version:
Etsuro Iwama, Pierre-Louis Taberna, Philippe Azais, Laurent Brégeon, Patrice Simon.
Character-ization of commercial supercapacitors for low temperature applications. Journal of Power Sources,
Elsevier, 2012, vol. 219, pp. 235-239. �10.1016/j.jpowsour.2012.07.029�. �hal-01153244�
OATAO is an open access repository that collects the work of Toulouse researchers and
makes it freely available over the web where possible.
This is an author-deposited version published in :
Eprints ID : 13893
To link to this article :
To cite this version :
Iwama, Etsuro and Taberna, Pierre-Louis and Azais, Philippe and
Brégeon, Laurent and Simon, Patrice Characterization of
commercial supercapacitors for low temperature applications.
(2012) Journal of Power Sources, vol. 219. pp. 235-239. ISSN
Any correspondance concerning this service should be sent to the repository
Characterization of commercial supercapacitors for low temperature applications
, P.L. Tabernaa,b
, P. Azaisc,1
, L. Brégeonc
, P. Simona,b,* aUniversité Paul Sabatier de Toulouse, CIRIMAT, UMR-CNRS 5085, 31062 Toulouse, Cedex 9, France
bRéseau sur le Stockage Electrochimique de l’Energie, (RS2E) FR CNRS n3459, France cBatscap, Groupe BOLLORE, Odet-Ergué-Gabéric, 29556 Quimper, Cedex 9, France
h i g h l i g h t s
Low temperature electrolytes were tested with commercial 600F SC cell.
Mixing MA enlarged low temperature limit of AN-based SC cell from40 to 55C. High temperature performance was exempliﬁed by ﬂoating at 2.7 V and þ60C.
Keywords: Supercapacitor Commercial cell
Low temperature electrolyte Methyl acetate
a b s t r a c t
Electrochemical characterizations at low temperature andﬂoating tests have been performed on 600F commercial supercapacitor (SC) for acetonitrile (AN)-based and ANþ methyl acetate (MA) mixed elec-trolytes. From40 to þ20C, AN electrolyte showed slightly higher capacitance than those of ANþ MA mixed electrolytes (25 and 33 vol.% of MA). At55C, however, AN electrolyte did not cycle at all, while MA mixed electrolyte normally cycled with a slight decrease in their capacitance. From electrochemical impedance spectroscopy measurements, the whole resistance for AN-based cells at55C was found to be about 10,000 times higher than that ofþ20C, while a 40-fold increase in the cell resistance was obtained for the MA mixture between 20 and55C. From the results ofﬂoating tests at 2.7 V and 60C for 1 month, the 25 vol.% MA mixture showed no change and slight decreased but stable capacitance.
The increasing importance of global environment deterioration and diminishing energy supplies are major factors prompting the introduction of electrical energy devices into transportations such as vehicles, trains, and airplanes. In aeronautics for these days, apart from driving energy of airplanes, other energy supplies such as for navigation, a landing and a wing operation, lightning, and air conditioning during their ﬂight become more and more indis-pensable. These auxiliary energy supplies depend on three energy systems, hydraulic, pneumatic, and electric. Recent investigations have been focused on replacing the former two systems with the
electric system due to its advantages of i) less fuel depending, ii) smaller maintenance cost, iii) simpler design, and iv) less contamination in environment[1,2]. For the aeronautics applica-tions (more electric aircraft; MEA), however, the required condition for the equipment is severe, especially for the energy device, which should be required to i) lightness of the device, ii) high power density iii) good cycleability, iv) credibility, and v) wide tempera-ture range[2,3].
Supercapacitors (SCs), also called as ultracapacitors or electrochemical capacitors, are energy devices, which store electric charges in an electrical double layer at carbon electrodeeelectrolyte interface. These devices provide higher power density (103e104 W kg1), medium energy density
(z5 Wh kg1), excellent cycleability (up to several millions), and relatively wider operational temperature range (40 < T < þ70C), compared to batteries based on slow and
temperature depending electrochemical reactions. Thanks to these safe and reliable properties, SC cells have been used for consumer electronics, memory back-up systems, industrial power and energy management, hybrid cars, catenary-free light
* Corresponding author. Université Paul Sabatier de Toulouse, CIRIMAT, UMR-CNRS 5085, 31062 Toulouse, Cedex 9, France. Tel.: þ33 561556802; fax: þ33 561556163.
E-mail addresses: email@example.com (L. Brégeon), simon@ chimie.ups-tlse.fr(P. Simon).
1Present address: CEA-LITEN, 17 rue des Martyrs, 38054 Grenoble, Cedex 9, France.
rail vehicles and even aeronautics such as emergency opening doors on the Airbus A380[6e10]. These reliable SC cells would be installed more and more into the MEA industry in the near future.
Generally, SC cells compose of two porous carbon electrodes attached on Al current collector and separated by porous membrane impregnated with an aqueous or nonaqueous lyte. From the viewpoint of energy density, nonaqueous electro-lytes which consist of tetraethylammonium tetraﬂuoroborate (TEABF4) with acetonitrile (AN) or propylene carbonate (PC) is
preferred to aqueous electrolyte, due to their wider voltage window. Conventional SCs using AN, however, have faced a critical problem due to the high melting point of AN (45C), considering
the required operation temperature for MEA application is at 55C. Using PC instead of AN leads much limitation of the use in
low temperature (>25 C) due to its lower ionic conductivity
[3,11]. To overcome this low temperature issue, several investiga-tions have been reported[3,12e17]. A. Jänes et al.ﬁrstly used the binary, ternary and quaternary mixture of ethylene carbonates and organic esters such as methyl acetate (MA), methyl formate (MF), and ethyl acetate (EA) for SC cells, and the certain mixtures showed the improved conductivity at low temperature than that of PC
[12,13]. E.J. Brandon et al. reported SC performances at low temperature, using AN mixed with EA, MA, MF, or 1,3-dioxolane
[3,14]. These co-solvents were chosen because of their low melting points, relatively low viscosity, and medium dielectric constants. Using triethylmethylammonium tetraﬂuorborate (TEMABFA4) or
spiro-(1,10)-bipyrrodium tetraﬂuoroborate (SBPBF4) in AN and MF
mixture solvents was also investigated[15,16]. Eutectic mixture of ionic liquids with exohedral carbons was recently reported as well
. These mixture electrolytes certainly showed promising char-acteristic enabling SC performance below the limit of temperature of AN45C.
In this study, we chose MA as a co-solvent of AN, because of its low melting temperature of98.0C and low viscosity of 0.364 cP
(Table 1). These electrolyte mixtures have been used in commercial 600 F 12 W SC cells manufactured by Batscap. Low temperature charge-discharge down to55C and the aging tests up to 60C
were achieved to check the interest of these electrolytes for MEA applications.
The low temperature measurements have been performed on a Batscap SC composed of activated carbon electrodes and an organic electrolyte with a nominal capacitance of 600 F, for temperatures between55 and þ20C. Tetraethylanmonium
ﬂu-oroborate (TEABF4, Acros Organics, 99%) was chosen as the
elec-trolytic salt. Solvents used were acetonitrile (AN, Acros Organics, 99þ%, extra dry < 50 ppm of water) and mixtures of AN and methyl acetate (MA, Alfa Aesar, 99%). Prepared electrolyte compositions were 1 M TEABF4in pure AN, ANþ MA (75:25 in volume), and
ANþ MA (67: 33). Electrolyte formulations were made in an argon-ﬁlled globe box (Braun, Unilab < 0.1 ppm of water and oxygen). Conductivity of the three electrolytes at different temperatures was measured by Zahner impedancemeter, in a two-electrodes Swa-gelok cell conﬁguration. Each cell was composed of two stainless steel electrodes (
f¼ 1.1 cm) and glass ﬁber separator (
f¼ 1.2 cm, Whatman GF/B). Batscap assembled commercial SC cells by using these electrolytes (Fig. 1(a)). The connection between SC cell and measurement cables with minimized contact resistance, and our test protocols are shown in Fig. 1(b) and (c), respectively. Chargeedischarge tests were performed for 10 cycles at each temperature,þ20, 20, 40 and 55C, with constant current of
3 A from 0 to 2.5 V controlled by Arbin (Arbin Instrument). In advance of the measurements, SC cells were stored for 6 h at each temperature in a controlled climatic chamber. After every 10 cycles, cell impedance has been measured at OCV with amplitude of 10 mV from 10 m to 100 kHz controlled by Zahner impedance spectrom-eter. Floating tests have been performed on the same Batscap SC cells at 2.5 and 2.7 V controlled by VMP3 (BioLogic), for tempera-tures betweenþ50 and þ60C. The cell impedance was measured
at each voltage with amplitude of 10 mV from 10 m to 100 kHz with VMP3, recorded every 24 h during 1 month.
3. Electrochemical characterizations
The measured conductivity data is shown in Fig. 2. The conductivity of the AN-based electrolyte in the studied T range is similar to those reported in the literature, with an expected decrease of conductivity with decreasing T. Since the temperature of55C was below the freezing point of the AN electrolyte, it was
impossible to measure conductivity. The conductivity for
Physical properties of acetonitrile and methyl acetate.
Acetonitrile Methyl acetate CH3C^N Tm/C 43.8 98.0 Tb/C 81.6 56.9 h/cP 0.341 0.364 ε/e 35.9 6.68 T / +20 -20 -40 -55
4Measurement sequence Storage for 6 hrs at each T, 10 cycles of charge discharge tests at T
EIS measurements at T
Fig. 1. Images of (a) assembled 600 F 12W SC cell and (b) connected SC cell with cables and (c) our test protocol.
mixed electrolytes was lower than those for the AN electrolyte. The value decreased with an increase in volume of MA from 25 to 33 vol.%, due to the lower dielectric constant of MA than AN as shown inTable 1. Unlike the AN electrolyte, MA-mixed electrolytes were still conductive at 55 C, showing the highest value of
9 mS cm1for the MA¼ 25 vol.%. The discharge curves at every 10th cycles for temperatures between55 and þ20C were shown
in Fig. 3. From 40 to þ20 C, curves for all three electrolytes
maintained their linear shapes, showing typical capacitive behavior
. At55C, the difference in the shape became clear with and
without MA. For the AN electrolyte, no charge discharge response was observed as shown inFig. 3(a). The vertical voltage drop is indicative of a large resistance for AN electrolyte. This result clearly shows that AN electrolyte doesn’t work at 55C, which is lower
than AN freezing point of45C. MA-mixed electrolytes, however,
maintained their linear shape with a slight decrease in their capacity (Fig. 3(b) and (c)). Thus, this result shows that mixing MA with AN decreases the freezing point of electrolyte mixture without any serious degradation of charge-discharge performances which was previously shown . The capacitance calculated from discharge curves is given in Fig. 4. From þ20 to 40 C, the capacitance for three electrolytes remains almost constant. The capacitance for AN electrolyte were slightly superior to those of MA-mixed electrolytes, while 25 vol.% MA mixture showed higher capacitance than 33 vol.%. At55C, as discussed above, AN
elec-trolyte showed no capacitance, while capacitance for 25 and 33 vol.% MA mixtures maintain 95 and 91% of the capacitance at 20C.
To investigate the change of the resistance components, elec-trochemical impedance spectroscopy (EIS) for three electrolytes at different temperatures were measured. For all the data, the connection resistance of cables was subtracted from real part impedance. As shown in Fig. 5(a), EIS spectra for AN electrolyte show typical EIS spectra of SC and remained same shape in the range between40 and þ20C. As expected, only the high
frequency resistance shifts to higher value while T decreased. At 55C, however, the large semi-circle was suddenly observed and
the whole resistance increased from 1.8 m
U. Appearance of the large semi-circle suggests a large reformation of interface
between electrolyte and electrode due to the crystallization of AN electrolyte. In comparison, resistance for MA-mixed electrolytes increases with a decrease of temperature from 20 to 55 C
(Fig. 5(b) and (c)). Below40C, even small semi-circle due to the
Fig. 2. Electrolyte conductivity vs. temperature for the three electrolytes studied, 1 M TEABF4in (B) AN, (6) ANþ MA (75:25) and (,) AN þ MA (67:33).
Fig. 3. Discharge curves for 1 M TEABF4in (a) AN, (b) ANþ MA (75:25 in volume) and (c) ANþ MA (67:33) at þ20, 20, 40 and 55C.
Fig. 4. Evaluated capacitance from discharge curves for 1 M TEABF4in (B) AN, (6) ANþ MA (75:25) and (,) AN þ MA (67:33) at þ20, 20, 40 and 55C.
modiﬁcation of the contact between electrode and electrolyte appeared. Unlike results of AN electrolyte, the increase of low frequency resistance at55C for MA-mixed electrolytes remains
acceptable with value from 0.07 to 0.11
U. Fig. 6(a) shows the change of resistance at 1 kHz (R@1KHz) with temperature, except
large value of R@1KHzfor AN electrolyte at55C (16.4
U). From 20
to55C, R@1KHzfor all 3 electrolytes increases with a decrease in
temperature. Furthermore, we evaluated ionic resistance (Rionic) in
porous carbons from EIS spectra and results were plotted in
Fig. 6(b). As shown in inlet ofFig. 6(b), Rionicwas calculated by
subtracting Rstartto Rend, and this allowed us to discuss the pure
resistance increase for different electrolyte. At þ20 C, the
order of Rionicwas 0.6 m
Ufor (c) MA¼ 33 vol.% > 0.4 m
MA¼ 25 vol.% > 0.2 m
Ufor (a) AN electrolyte. Higher Rionicfor the
MA mixtures is due to a decrease in ionic conductivity by mixing MA as shown inFig. 2. The order was same until down to40C
and the Rionicfor (a) increased very slightly from 0.2 to 0.5 m
while that for (b) was from 0.4 to 3.6 m
U, and that for (c) was from
0.6 to 7 m
U. This order of Rioniccorresponds to the measured
conductivity at40C as well. At55C, the Rionicfor AN
elec-trolyte was not evaluable due to the large EIS spectra change, while the value was minimized to 36 m
Ufor (b) MA¼ 25 vol.%. This clearly shows that MA¼ 25 vol.% mixture was superior at 55C
chargeedischarge operation, due to the low resistance of ionic resistance in the carbon pores (Fig. 3).
Floating tests at high temperature at the temperature between 50 and 60C for 4 weeks (1 month) were performed with an SC cell composed of 25 vol.% MA-mixed electrolytes, since we were aware of the concern of low boiling point of MA (56.9 C) compared to that of AN (81.6C).Fig. 6(a) shows EIS spectra for the SC cell ﬂoated at 2.7 V, 60 C during 1 month. No obvious
change can be seen in the shape of EIS spectra. These results clearly show that equivalent series resistance (ESR) of the cell for 25 vol.% MA mixed electrolyte remained constant even under severe high temperature 60 C and high voltage 2.7 V. The capacitance C of ﬂoated SC were evaluated from the following equation; C¼ 1/(2
pfZ00), where f is the frequency and Z00is the corresponding imaginary impedance. Obtained capacitance for difference temperature and voltage were plotted inFig. 7(b). After 1 week, slight decrease in capacitance was observed from the initial capacitance for every 3 conditions. Even though there is difference in capacitance for 3 conditions, the values of capaci-tance retention (¼Capacitance/Capacitance at 0 week) are same. After 2 weeks their capacitance remained almost stable until the end ofﬂoating tests. These results show that the SC 600 F cells 25 vol.% mixing of MA endured during the 4 weeksﬂoating tests at high temperatures.
Fig. 5. Niquist plots measured at OCV for 1 M TEABF4in (a) AN, (b) ANþ MA (75:25) and (c) ANþ MA (67:33) at þ20, 20, 40 and 55C. Amplitude was 10 mV and the frequency range was from 10 m to 100 kHz.
Fig. 6. (a) change of resistance at 1 kHz (R@1kHz) with temperature and (b) ionic resistance in carbon pores estimated from ESI results for 1 M TEABF4in (B) AN, (6) ANþ MA (75:25) and (,) AN þ MA (67:33) at þ20, 20, 40 and 55C.
Mixing MA into conventional AN-based electrolyte successfully enlarged the low temperature operation range of commercial 600F
SC cells from40 to 55C. After the modiﬁcation of MA mixing
composition, 25 vol.% of MA mixture was slightly superior to the 33 vol.% MA mixture. These 25 vol.% MA mixtures can operate at high temperature as well, exempliﬁed by ﬂoating tests at 2.7 V andþ60C for 1 month.
The work reported here wasﬁnancially supported by the French project named as“Réseau local d’alimentation et de RÉCUPération d’ENERgie à bord (RÉCUPENER).
 O. Langlois, E. Foch, X. Roboam, H. Piquet, J3eA 4 (2005) 1.  A. Griffo, J. Wang, Elect. Power Syst. Res. 82 (2012) 59.
 E.J. Brandon, C. William, M.C. Smart, L.D. Whitcanack, A. Gary, A. Plett, J. Power Sources 170 (2007) 225.
 P. Simon, Y. Gogotsi, Nat. Mater. 7 (2008) 845.  J.R. Miller, P. Simon, Science 321 (2008) 651.
 http://www.citroen.fr/technologie-ehdi/#/technologie-ehdi/(accessed 06.04.12).  http://www.peugeot.com.au/media/deliacms/media/19/1935-4fbb65.pdf
 L.L. Zhang, X.S. Zhao, Chem. Soc. Rev. 38 (2009) 2520.
 Q. Cheng, J. Tang, J. Ma, N. Shinya, L.C. Qin, Phys. Chem. Chem. Phys. 13 (2011) 17615.
 V. Presser, M. Heon, Y. Gogotsi, Adv. Funct. Mater. 21 (2011) 810.
 M. Arulepp, L. Permann, J. Leis, A. Perkson, K. Rumma, A. Jänes, E. Lust, J. Power Sources 133 (2004) 320.
 A. Jänes, E. Lust, Electrochem. Commun. 7 (2005) 510.  A. Jänes, E. Lust, J. Electroanal. Chem. 588 (2006) 285.
 E.J. Brandon, M.C. Smart, W. West, Nasa Tech. Briefs 32 (2008) 32.  E.J. Brandon, M.C. Smart, C. William, Nasa Tech. Briefs 34 (2011) 44.  Y. Korenblit, A. Kajdos, W.C. West, M.C. Smart, E.J. Brandon, A. Kvit, J. Jagiello,
G. Yushin, Adv. Funct. Mater. 22 (2012) 1655.
 R. Lin, P.L. Taberna, S. Fantini, V. Presser, C.R. Perez, F. Malbosc, N.L. Rupesinghe, K.B.K. Teo, Y. Gogotsi, P. Simon, J. Phys. Chem. Lett. 2 (2011) 2396.
 A. Balducci, R. Dugas, P.L. Taberna, P. Simon, D. Ple, M. Mastragostino, S. Pass, J. Power Sources 165 (2007) 922.
 B.E. Conway, Electrochemical Supercapacitors: Scientiﬁc Fundamentals and Technological Applications, Kluwer-Plenum, New York, 1999.
Fig. 7. (a) Niquist plots for 1 M TEABF4in ANþ MA (75:25) at 2.7 V and þ60C for 1 month. (b) Evaluated capacitance for 1 M TEABF4in ANþ MA (75:25) at (B) 2.5 V and 50C, (6) 2.5 V and 60C, and (,) 2.7 V and þ60C for 1 month.